Structure and Properties of Functionalized Porous Silica Hybrid
Open Journal of Inorganic Non-Metallic Materials, 2014, 4, 35-43
Published Online July 2014 in SciRes. http://www.scirp.org/journal/ojinm
Structure and Properties of Functionalized
Porous Silica Hybrid Materials
Elena V. Todorova, Georgi E. Chernev, Stoqn P. Djambazov
Department “Silicate technology”, University of Chemical Technology and Metallurgy, Sofia, Bulgaria
Email: [email protected]
Received 20 May 2014; revised 19 June 2014; accepted 17 July 2014
Copyright © 2014 by authors and Scientific Research Publishing Inc.
This work is licensed under the Creative Commons Attribution International License (CC BY).
Functionalized silica hybrid materials are extensively studied and applied materials in the field of
science and technology. Functionalization is an approach, which allows for the application of organic components in the improvement of the design, properties and potential application of silicate materials. Silica hybrid materials, functionalized via incorporation of organic components
(chitosan and methacrylic acid) were synthesized by the sol-gel method. The base silica structure
of the hybrids was obtained via hydrolysis and condensation of the silicate precursor, tetraethyl
orthosilicate. The investigations of synthesized hybrids are focused on the influence of the nature
and quantity of functional organic components on their final structures and properties. The structural characteristics of obtained hybrid materials were investigated using XRD, FTIR, SEM and
DTA/TG analysis. The obtained results presented the formation of amorphous porous structure
and the organic components are evenly distributed into the silica network. The functional radicals
of chitosan and methacrylic acid (amine, hydroxyl groups) exist in the hybrid structure as free
reactive centers, as their quantity increases with increasing the organic amount. The swelling behavior in acidic and neutral solutions of the synthesized materials is investigated and the results
presented, that the silicate materials exhibit hydrophilic character.
Sol-Gel, Silica Hybrids, Functionalization, Porosity, Biomaterials
Science and technology leads to the improvement of materials, which are able to cater for present and pressing
needs. Hybrid materials play an important role for this purpose due to the possibility of combining suitable
properties in one structure. These materials should cover the application requirements, as well as be accessible,
reusable and cost-effective  .
How to cite this paper: Todorova, E.V., Chernev, G.E. and Djambazov, S.P. (2014) Structure and Properties of Functionalized
Porous Silica Hybrid Materials. Open Journal of Inorganic Non-Metallic Materials, 4, 35-43.
E. V. Todorova et al.
Synthesis of hybrid materials with diverse properties can be achieved via a modification of inorganic structure
with organic components. The proposed system can combine inorganic stability and durability with plasticity
and specific properties normally associated with organic materials. Functionalization of the inorganic structure
is an approach, which allows for obtaining hybrid materials with improved behavior and application  .
Functional hybrids can successfully be applied in any field, which requires contact interactions on the surface
(environmental remediation, immobilization of biomolecules, etc.) -.
Important determinants in the development of functional hybrids are the preparation technique(s) and precursor material behavior. Requirements such as low-cost, easy preparation and accessible equipment also reduce
the variety of synthesis routes. One route, which covers all of the above requirements, is that of sol-gel synthesis.
This technique allows preparation of different compositions, independently of the state (amorphous, crystal),
which is required, as well as controlling each step of the process . Most of the materials, whose structures can
easily be modified with different functional radical, and prepared via sol-gel synthesis, are silicates  .
The silicates are inorganic components, which can easily be transformed from precursor into monolith, porous,
thin film or coating material. Silica materials possess high thermal resilience and can withstand high pressures
and external aggressive materials and media  . Regardless of the silica stability their application is limited, due to reduce pollutant reactivity and degradability. Therefore, a combination with suitable organic components serves as a great opportunity to improve the plasticity and stability of the silica structure, and to improve
contact behavior with external moieties .
Acrylates are synthetic organic components known as good film formers, with high mechanical stability 
. In polymerized form, acrylates have been proven to be excellent protective materials, but limitations such
as poor water and temperature resistance reduces their potential applications. Combinations of acrylate with silica components allow for the formation of hybrids with improved long-term stability and durability . The
application of these hybrid materials is connected to the free reactive groups of the acrylate. Acrylates with long
chain structures or further polymerization have fewer free reactive centers and a consequently reduced potential
application. Furthermore, the hydrophilicity also decreases when the acrylate chain is longer and this causes an
unfavorable effect on possible interactions with external molecules . Methacrylic acid is a suitable acrylate
which in combination with silica material will lead to the realization of a hybrid with improved stability, resistance and available functional groups. The structure of this organic material contains carboxylic group, which
can be dissociated into C3H5COO− anion and H+ cation. In addition the carboxyl groups can easily interact with
amine functionalized biomolecules for immobilization purposes or cationic pollutants (heavy metals). Addition
of MA into silica network leads to the formation of a hybrid with improved functionality and hydrophilicity 
. Nevertheless the variety of high functionalized centers is limited due to the dissociation possibility of carboxylic groups in different media, as well as contact only with cationic molecules  . Preparation of silica
hybrid material with improved functionalized surface and the ability to interact with different types of external
molecules can be obtained with a combination of another organic component .
Natural organic components are suitable materials, due to their biocompatibility, degradability, non-toxicity
and abundance. The investigations focused on preparation of functional materials for environmental or immobilization purposes established that the existence of free amine groups play an important role in interactions with
external moieties like waste water pollutants or biomolecules. One of the most abundant natural organic materials is chitosan, whose structure contains free amine and hydroxyl groups, which act as reactive centers . In
acidic solutions, the attraction process with pollutants is increased from protonation of amine groups .
The preparation of a silica network matrix into which the organic components (chitosan and methacrylic acid)
are evenly distributed as separate units can lead to the formation of an innovative hybrid material with improved
functionality. The use of the full qualities of the organic components allows for the formation of a material suitable for different pollutants/biomolecules.
Silica hybrid materials, modified by addition of chitosan and methacrylic acid organic components were synthesized via the sol-gel method. Characterization of the structure by XRD, FTIR, SEM and DTA/TG analysis
was conducted to determine the structural nature of the hybrid material, as well as the influence of the used
2. Materials and Methods
Tetraethyl orthosilicate (TEOS, 98%, Sigma Aldrich), chitosan (CS, degree of deacetylation 75% - 85%, Fluka),
E. V. Todorova et al.
methacrylic acid (MA, Fluka), dH2O, HCl (37%, Merck) and acetic acid (99%, Sigma Aldrich) were the initial
components for preparation of the innovative silica hybrid materials.
2.2. Synthesis Procedure
Functionalized hybrid materials based on silicates with participation of organic components (CS and MA) was
synthesized via the sol-gel method. The first step of the preparation process is the hydrolysis of the silica source
(TEOS) using d H2O, and HCl as a catalyst. After mixing the components and stirring with a magnetic stirrer for
1h, a silica sol is obtained. For better distribution and compatibility of CS in the hybrid structure this polysaccharide was dissolved in 1% acetic acid. After complete dissolution (30 min via vigorous stirring), a calculated
amount of CS solution was added to the silica sol. Immediately after the addition of CS, an equal amount of MA
was added and the solution was stirred for another 30 min. The obtained homogeneous sols were poured onto
Petri dishes, where the hybrid material transformed into gels. The realized gels were then dried at room temperature. To establish the compatibility of the used components, and the influence of organic components on hybrid
structures, five samples with different organic quantities were synthesized: TEOS/CS/MA = 1:0.1:0.1 (SiCSMA1); TEOS/CS/MA = 1:0.2:0.2 (SiCSMA2); TEOS/CS/MA = 1:0.3:0.3 (SiCSMA3); TEOS/CS/MA =
1:0.4:0.4 (SiCSMA4); TEOS/CS/MA = 1:0.5:0.5 (SiCSMA5).
2.3. Structural Characterization
The structural characteristics of the synthesized hybrid materials are crucial in determining their suitability for
their intended application. XRD (Brucker D8 Advance; Cu-Kα radiation with scan rate of 0.020.min−1 in 2θ
range between 100 and 800.) was used to determine the state of the obtained hybrid materials. The specific
groups of used components and chemical bonds formed via sol-gel synthesis were observed via FTIR analysis
(MATTSON 7000, BRUKER TENSOR 27 Spectrometer, 4000 - 400 cm−1). SEM (Hitachi SU-70) analysis was
used for observation of prepared silica hybrid structures. For understanding the thermal stability of obtained hybrids DTA/TG (Setaram LabsysTm TG-DSC16, temperature diapason 0˚C - 1000˚C, heating rate 10˚C/min)
analysis was used.
2.4. Swelling Measurement
To establish the influence of the CS and MA organic components on the properties of the synthesized silica hybrid materials their swelling behavior in different media (acidic (1 M HCl, pH = 3) and distilled water (pH = 7)
solutions) was analyzed. Obtained silica hybrid materials with known weight (M1) were immersed in the solutions (10 ml) at an ambient temperature for 24 h. Afterwards, the samples were removed, dried and measured
again (M2). The weight change percentage (W, %) was calculated according to the Equation (1) :
M2 − M1
3. Results and Discussion
The state of the synthesized hybrid materials was evaluated via XRD analysis. The results (Figure 1) showed
presence of wide range peak around 23 2θ and low intensive peak ~12 2θ. Preparation of hybrid materials based
on TEOS and using sol-gel synthesis at room temperature lead to the formation of a silica network in an
amorphous state. XRD patterns proved the formation of amorphous silica structure with presence of wide range
peak around 23 2θ. The organic component chitosan can exist in three different forms-noncrystalline (11.7 2θ),
hydrated crystalline (14.2 2θ) and anhydrous crystalline (23 2θ) . The peak around 12 2θ showed that added
CS is in amorphous form.
The establishment of the structural groups in the obtained hybrid materials via FTIR analysis gives information about the influence of the used preparation technique and component behaviour (Figure 2(a)). Intensive
peaks at 450 and 550, as well as 1090 cm−1 are associated with silica symmetric and asymmetric stretching vibrations, respectively. Presence of characteristic Si-O-Si bonds showed the successful formation of a hybrid
material on the silica based of network. Existence of free Si-OH groups associated with the peak at 950 cm−1 are
due to incomplete condensation reaction of available silanol units . Free hydroxyl groups play favourable
E. V. Todorova et al.
Figure 1. XRD patterns of obtained silica hybrid materials.
Figure 2. FTIR spectra (a) and model structure (b) of synthesized silica hybrid materials.
affect on the functionality of prepared silica hybrid materials. Another characteristic peaks for sol-gel synthesis
at room temperature are of water molecules and on the FTIR spectra corresponding to the peaks at 1640 and the
wide range peak at 3400 cm−1. Characteristic peaks of used organic components are also observed on FTIR
spectra of synthesized hybrids. The peak around 1200 cm−1 is assigned to the asymmetric stretching of C-O-C
bridge chain of chitosan . Symmetric deformations of -CH3 and -CH2 groups of CS and MA are assigned
with the peaks at 1460 and 2980 cm−1 . Existences of characteristic free reactive groups of CS (N-H and
-OH) are associated with peaks at 1520 and in the range 3400 cm−1 . Specific C = C group of MA structure
is associated with peak at 1640 cm−1. Functional carboxylic group of synthetic organic component is associated
with the peak at 1710 cm−1 .
FTIR spectra showed that the synthesized hybrid materials are based on silica network into which the organic
components are successfully incorporated. Hydroxyl, carboxyl and amine groups, which were found to be existent in the hybrid structures proved, that the synthesized innovative hybrids can be applied for immobilization
purposes or used as protective materials. The free reactive centres allows for interactions with cationic and anionic external moieties. Model structure and possible interactions between the used components of obtained silica
E. V. Todorova et al.
hybrid materials is shown on Figure 2(b).
The structure of the obtained silica hybrid materials was observed via SEM analysis (Figure 3). Different
structures with varying porosities were obtained as a result of the variation of the compositions of the organic
components. The obtained micrographs presented formation of homogeneous materials due to preparation of
silica network with pores all over the entire structure as a result of used MA component . The pore size of
SiCSMA1 samplel varied between 4 and 10 μm. With an increasing of the amount of organic component, the
pore size increased up to 50 μm (SiCSMA5), and their quantity decreased.
The obtained results from SEM analysis posses influence of organic nature on the final structures. The organic components added into the hybrid materials lead to the formation of porous structures with improve functional contact surface area. For preparation of high reactive materials, which can easily attract and interact with external molecules, MA and CS are suitable candidates for that purpose.
The behavior of the obtained hybrid materials during thermal treatment was determined using DTA analysis.
TG analysis showed weight loss of the hybrids through the temperature diapason 0˚C - 1000˚C. For a better un-
Figure 3. SEM micrographs of obtained silica hybrid surfaces.
E. V. Todorova et al.
derstanding of the influence of CS and MA on the structure and properties of hybrid materials, sample SiCSMA5 and pure silica were tested (Figure 4).
DTA thermograph of pure silica sample showed intensive endothermic reaction around 130˚C. The endothermic reaction is correlated to the evaporation of adsorbed and chemically bonded water molecules. This can
be proved with drastically weight loss in the temperature diapason 50˚C - 200˚C. After 130˚C condensation of
silanol units and self-compacting of the hybrid material is observed. Maximum weight loss of pure silica material established from TG analysis is 22%. The obtained weight loss results clearly demonstrated the effect of the
preparation technique-sol-gel synthesis at room temperature (Figure 4(a)).
The DTA/TG curves for sample SiCSMA5 presented intensive endothermic reaction around 105˚C and
weight loss 30% (Figure 4(b)). The reduce temperature of the reaction is associated with addition of organic
components in the silica material, which leads to decreasing of the thermal stability. The reaction occurred with
lower thermal energy due to the big quantity of organic components. Furthermore, the results presented, that the
CS and MA units are located on the hybrid surface and their degradation is favored. Maximum weight loss
(30%) is associated with evaporation of adsorbed water molecules and degradation of organic components.
The swelling behavior of the synthesized porous hybrids was tested via weight change percentage (W, %) by
immersion in acidic and neutral solutions and the obtained results are presented on Figure 5. The results of
swelling test showed the different behavior of the synthesized hybrid structures by variation of pH.
In acidic and neutral solutions the weight change percent of pure silica is 2.96% and 2.03%, respectively. The
weight change of the pure silica presented the low hydrophilicity of the silica network. The attraction of the water molecules activated by silanol groups (Si-OH) kept due to the sol-gel synthesis at room temperature .
The addition of organic components led to improving the swelling behavior due to formation of porous materials
with improves contact surface area (established via SEM micrographs). Furthermore, the hydrophilic character
of the used organic components, as well as functional reactive centers (established via FTIR spectra) improve
the contact with the water molecules . Functional carboxylic groups of MA dissociated into COO-anion and
H+ cation . Hydroxyl and amine groups of CS, as well as-OH groups bonded with Si atoms also attract the
water molecules, as a result of which the weight increase. In acidic media the W values are higher, than these of
hybrid weight in neutral solution and can be associated with swelling behavior of CS units into solutions with
different pH . In acidic conditions the CS units expanded, as a result of which penetration of water molecules is, favor . In both media the swelling tests presented that with increasing of the organic amount the
weight of the hybrid materials also increase. The results showed that the functionalization of silica network
(known as hydrophobic material) play important role for further application of the synthesized hybrids . The
organic components, which are proven as hydrophilic materials improve the hydrophilicity of the hybrid structures, which plays favorable effect on the interactions with external molecules -.
Figure 4. DTA/TG curves of pure silica (a) and SiCSMA5 hybrid material (b).
E. V. Todorova et al.
Figure 5. Results of swelling test of the synthesized silica hybrid materials.
Porous hybrid materials with functional surfaces were obtained via incorporation of CS and MA in a silica network. Functionalized silica materials synthesized by the sol-gel technique are amorphous with large surface
contact area and exhibit hydrophilicity and thermal stability. The obtained hybrid materials showed good stability in acidic and neutral solutions, where the functional units as free reactive centers can interact with external
moieties. The investigations of the structure and properties of synthesized silica/CS/MA materials showed, that
these functionalized hybrids can be successfully applied for the immobilization of different biomolecules or as
adsorbents of pollutants.
This material has been published with the support of a project BG051PO001/3.3-05-001 “Science and business”,
financed by Operational programme “Human Resources Development” to European Social Fund.
Lee, K., Morad, N., Teng, T. and Poh, B. (2012) Development, Characterization and the Application of Hybrid Materials in Coagulation/Flocculation of Wastewater: A Review. Chemical Engineering Journal, 203, 370-386.
Xia, K., Ferguson, R., Losier, M., Tchoukanova, N., Brüning, R. and Djaoueda, R. (2010) Synthesis of Hybrid Silica
materials with Tunable Pore Structures and Morphology and Their Application for Heavy Metal Removal from Drinking Water. Journal of Hazardous Materials, 183, 554-564. http://dx.doi.org/10.1016/j.jhazmat.2010.07.060
Wang, T., Chen, Y., Ma, Y., Chen, M., Nie, C., Hu, M., Li, Y., Jia, Z., Fang, J. and Gao, H. (2013) Ampholine-Functionalized Hybrid Organic-Inorganic Silica Material as Sorbent for Solid-Phase Extraction of Acidic and Basic Compounds. Journal of Chromatography A, 1308, 63-72. http://dx.doi.org/10.1016/j.chroma.2013.08.025
Miao, T. and Wang, L. (2007) Immobilization of Copper in Organic-Inorganic Hybrid Materials: A Highly Eﬃcient
and Reusable Catalyst for the Ullmann Diaryl Etheriﬁcation. Tetrahedron Letters, 48, 95-99.
Hu, Y., Tang, S., Jiang L., Zou, B., Yang, J. and Huang, H. (2012) Immobilization of Burkholderia Cepacia Lipase on
Functionalized Ionic Liquids Modiﬁed Mesoporous Silica SBA-15. Process Biochemistry, 47, 2291-2299.
E. V. Todorova et al.
Crippa, M., Callone, E., D’Arienzo, M., Müller, K., Polizzi, S., Wahba, L., Morazzoni, F. and Scotti, R. (2011) TiO2
Nanocrystals Grafted on Macroporous Silica: A Novel Hybrid Organic-Inorganic Sol-Gel Approach for the Synthesis
of Highly Photoactive Composite Material. Applied Catalysis B: Environmental, 104, 282-290.
Tang, H., Guo, J., Sun, Y., Chang, B., Ren, Q. and Yang, W. (2011) Facile Synthesis of pH Sensitive Polymer-Coated
Mesoporous Silica Nanoparticles and Their Application in Drug Delivery. International Journal of Pharmaceutics, 421,
O’Brien, S., Copuroglu, M. and Crean, G.M. (2007) Effects of Refractive Index Modifiers and UV Light on an Epoxyfunctional Inorganic-Organic Hybrid Sol-Gel Derived Thin Film System. Applied Surface Science, 253, 7969-7972.
Liu, J., Xu, S. and Yan, B. (2011) Photoactive Hybrids with the Functionalized Schiff-Base Derivatives Covalently
Bonded Inorganic Silica Network: Sol-Gel Synthesis, Characterization and Photoluminescence. Colloids and Surfaces
A: Physicochemical Enineering Aspects, 373, 116-123. http://dx.doi.org/10.1016/j.colsurfa.2010.10.036
 Yen, M. and Kuo, M. (2012) Sol-Gel Synthesis of Organiceinorganic Hybrid Materials Comprising Boehmite, Silica,
and Thiazole Dye. Dyes and Pigments, 94, 349-354.
 Hasanzadeh, M., Shadjou, N., Eskandani, M. and Guardia, M. (2012) Mesoporous Silica-Based Materials for Use in
Electrochemical Enzyme Nanobiosensors. Trends in Analytical Chemistry, 40, 106-118.
 Hao, J., Han, M., Wang, C. and Meng, X., Enhanced Removal of Arsenite from Water by a Mesoporous Hybrid Material-Thiol-Functionalized Silica Coated Activated Alumina. Microporous and Mesoporous Materials, 124, 1-7.
 Wang, D., Zhang, J., Tian, X., Liu, D. and Sumathy, K. (2014) Progress in Silica Gel-Water Adsorption Refrigeration
Technology. Renewable and Sustainable Energy Reviews, 30, 85-104. http://dx.doi.org/10.1016/j.rser.2013.09.023
 Yuan, Y., Liu, R., Wang, C., Luo, J. and Liu, X. (2014) Synthesis of UV-Curable Acrylate Polymer Containing Sulfonic Groups for Anti-Fog Coatings. Progress in Organic Coatings, in press.
 Nollenberger, K. and Albers, J. (2013) Poly(meth)acrylate-Based Coatings. International Journal of Pharmaceutics,
457, 461-469. http://dx.doi.org/10.1016/j.ijpharm.2013.09.029
 Liao, W., Qu, J., Li, Z. and Chen H. (2010) Preparation of Organic/Inorganic Hybrid Polymer Emulsions with High
Silicon Content and Sol-Gel-Derived Thin Films. Chinese Journal of Chemical Engineering, 18, 156-163.
 Liu, J., Ma, J., Bao, Y., Zhu, Z., Zhang, J. and Ma, J. (2011) Effect of Long-Chain Acrylate on the Properties of Polyacrylate/Nano-SiO2 Composite Leather Finishing Agent. Polymer-Plastics Technology and Engineering, 50, 1546-1551.
 Mitchell, J.S. (2011) Spin-Coated Methacrylic Acid Copolymer Thin Films for Covalent Immobilization of Small Molecules on Surface Plasmon Resonance Substrates. European Polymer Journal, 47, 16-23.
 Sevšek, U. and Krajnc, P. (2012) Methacrylic Acid Microcellular Highly Porous Monoliths: Preparation and Functionalisation. Reactive & Functional Polymers, 72, 221-226. http://dx.doi.org/10.1016/j.reactfunctpolym.2012.02.007
 An, F., Feng, X. and Gao, B. (2010) Adsorption Property and Mechanism of Composite Adsorbent PMAA/SiO2 for
Aniline. Journal of Hazardous Materials, 178, 499-504. http://dx.doi.org/10.1016/j.jhazmat.2010.01.109
 Panic, V.V., Madzarevic, Z.P., Volkov-Husovic, T. and Velickovic, S.J. (2013) Poly(Methacrylic Acid) Based Hydrogels as Sorbents for Removal of Cationic Dye Basic Yellow 28: Kinetics, Equilibrium Study and Image Analysis. Chemical Engineering Journal, 217, 192-204. http://dx.doi.org/10.1016/j.cej.2012.11.081
 Anirudhan, T.S. and Rijith, S. (2012) Synthesis and Characterization of Carboxyl Terminated Poly(Methacrylic Acid)
Grafted Chitosan/Bentonite Composite and Its Application for the Recovery of Uranium(VI) from Aqueous Media.
Journal of Environmental Radioactivity, 106, 8-19. http://dx.doi.org/10.1016/j.jenvrad.2011.10.013
 Kwok, K.S., Koong, L.F., Chen, G. and McKay, G. (2014) Mechanism of Arsenic Removal Using Chitosan and Nanochitosan. Journal of Colloid and Interface Science, 416, 1-10. http://dx.doi.org/10.1016/j.jcis.2013.10.031
 Khalek, M.D., Mahmoud, G.A. and El-Kelesh, N.A. (2012) Synthesis and Characterization of Poly-Methacrylic Acid
Grafted Chitosan-Bentonite Composite and Its Application for Heavy Metals Recovery. Chemistry and Materials Research, 2, 1-12.
 Song, R., Xue, R., He, L., Liu, Y. and Xiao, Q. (2008) The Structure and Properties of Chitosan/Polyethyleneglycol/Silica Ternary Hybrid Organic-Inorganic Films. Chinese Journal of Polymer Science, 26, 621-630.
E. V. Todorova et al.
 Lee, E., Jun, S., Kim, H., Kim, H., Koh, Y. and Jang, J. (2010) Silica Xerogel-Chitosan Nano-Hybrids for Use as Drug
Eluting Bone Replacement. Journal of Material Science: Material Medicine, 21, 207-214.
 Sivakami, M.S., Gomathi, T., Venkatesan, J., Jeong, H., Kim, S. and Sudha, P.N. (2013) Preparation and Characterization of Nano Chitosan for Treatment Wastewaters. International Journal of Biological Macromolecules, 57, 204-212.
 Abdel-Raouf, M.E., Abdul-Raheim, A.M., El-Kafrawy, A.F., Maysour, N.E., Ibraheim, A.K. and Abdel-Azim, A.A.
(2013) PHEMA Magnetic Nanogels for Removal of Cu(II) Ions from Aqueous Solution. International Journal of Chemistry and Material Science, 1, 36-44.
 Kyzas, G.Z. and Lazaridis, N.K. (2009) Reactive and Basic Dyes Removal by Sorption onto Chitosan Derivatives.
Journal of Colloid and Interface Science, 331, 32-39. http://dx.doi.org/10.1016/j.jcis.2008.11.003
 Mahmoodian, H., Moradi, O. and Shariatzadeh, B. (2014) Grafting Chitosan and PolyHEMA on Carbon Nanotubes
Surfaces: “Grafting to” and “Grafting from” Methods. International Journal of Biological Macromolecules, 63, 92-97.
 Deng, W., Li, R., Zhang, M., Gong, L. and Kan, C. (2010) Inﬂuences of MAA on the Porous Morphology of P(StMAA) Latex Particles Produced by Batch Soap-Free Emulsion Polymerization Followed by Stepwise Alkali/Acid
Post-Treatment. Journal of Colloid and Interface Science, 349, 122-126. http://dx.doi.org/10.1016/j.jcis.2010.05.033
 Purcar, V., Stamatin, I., Cinteza, O., Petcu, C., Raditoiu, V., Ghiurea, M., Miclaus, T. and Andronie, A. (2012) Fabrication of Hydrophobic and Antireflective Coatings Based on Hybrid Silica Films by Sol-Gel Process. Surface and
Coatings Technology, 206, 4449-4454. http://dx.doi.org/10.1016/j.surfcoat.2012.04.094
 Zhang, J., Wang, L. and Wang, A. (2007) Preparation and Properties of Chitosan-g-Poly(Acrylic Acid)/Montmorillonite Superabsorbent Nanocomposite via in Situ Intercalative Polymerization. Industrial and Engineering Chemistry Research, 46, 2497-2502. http://dx.doi.org/10.1021/ie061385i
 Liu, Y., Liu, W., Chen, W., Sun, L. and Zhang, G. (2007) Investigation of Swelling and Controlled-Release Behaviors
of Hydrophobically Modified Poly(Methacrylic Acid) Hydrogels. Polymer, 48, 2665-2671.
 de Moura, M., Aouada, F. and Mattoso, L. (2008) Preparation of Chitosan Nanoparticles Using Methacrylic Acid.
Journal of Colloid and Interface Science, 321, 477-483. http://dx.doi.org/10.1016/j.jcis.2008.02.006
 Neto, B., Mata, A., Lopes, M., Rossi-Bergmannd, B. and Ré, M. (2014) Preparation and Evaluation of Chitosan-Hydrophobic Silica Composite Microspheres: Role of Hydrophobic Silica in Modifying Their Properties. Power Technology, 225, 109-126. http://dx.doi.org/10.1016/j.powtec.2013.10.046
 Zou, H., Wu, S. and Shen, J. (2008) Polymer/Silica Nanocomposites: Preparation, Characterization, Properties, and
Applications. Chemical Reviews, 108, 3893-3957. http://dx.doi.org/10.1021/cr068035q
 Treccani, L., Klein, T., Meder, F., Pardun, K. and Rezwan, K. (2013) Functionalized Ceramics for Biomedical, Biotechnological and Environmental Applications. Acta Biomaterialia, 9, 7115-7150.
 Copello, G., Mebert, A., Raineri, M., Pesenti, M. and Diaz, L. (2011) Removal of Dyes from Water Using Chitosan
Hydrogel/ SiO2 and Chitin Hydrogel/SiO2 Hybrid Materials Obtained by the Sol-Gel Method. Journal of Hazardous
Materials, 186, 932-939. http://dx.doi.org/10.1016/j.jhazmat.2010.11.097
 Zou, H., Wu, S. and Shen, J. (2008) Polymer/Silica Nanocomposites: Preparation, Characterization, Properties, and
Applications. Chemical Reviews, 108, 3893-3957.
Scientific Research Publishing (SCIRP) is one of the largest Open Access journal publishers. It is
currently publishing more than 200 open access, online, peer-reviewed journals covering a wide
range of academic disciplines. SCIRP serves the worldwide academic communities and contributes
to the progress and application of science with its publication.
Other selected journals from SCIRP are listed as below. Submit your manuscript to us via either
[email protected] or Online Submission Portal.